#------------------------------------------------------------------------------
#$Date: 2024-04-18 18:56:43 +0300 (Thu, 18 Apr 2024) $
#$Revision: 291269 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/03/9000356.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9000356
loop_
_publ_author_name
'Smyth, J. R.'
_publ_section_title
;
 An orthopyroxene structure up to 850 C
 T = 500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              636
_journal_page_last               648
_journal_volume                  58
_journal_year                    1973
_chemical_formula_sum            'Ca0.032 Fe1.332 Mg0.635 O6 Si2'
_chemical_name_mineral           Ferrosilite
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.429
_cell_length_b                   9.028
_cell_length_c                   5.26
_cell_formula_units_Z            8
_cell_volume                     875.143
_database_code_amcsd             0000365
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.693
_cod_original_formula_sum        'Si2 Mg.635 Fe1.332 Ca.032 O6'
_cod_database_code               9000356
loop_
_space_group_symop_operation_xyz
x,y,z
x,1/2-y,1/2+z
-x,1/2+y,1/2-z
1/2-x,1/2+y,z
1/2+x,1/2-y,-z
1/2+x,y,1/2-z
1/2-x,-y,1/2+z
-x,-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
Sia 0.27190 0.33920 0.05720 1.00000
Sib 0.47450 0.33620 0.78740 1.00000
Mg1 0.37520 0.65320 0.88410 0.57600
Fe1 0.37520 0.65320 0.88410 0.42300
Fe2 0.37720 0.48500 0.37770 0.90900
Mg2 0.37720 0.48500 0.37770 0.05900
Ca2 0.37720 0.48500 0.37770 0.03200
O1a 0.18410 0.33770 0.05220 1.00000
O2a 0.31200 0.49520 0.06840 1.00000
O3a 0.30190 0.23740 -0.17780 1.00000
O1b 0.56270 0.33840 0.78590 1.00000
O2b 0.43450 0.48310 0.70310 1.00000
O3b 0.44810 0.21120 0.57570 1.00000
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0000365
